Order-disorder (OD) polytypism of K<sub>3</sub>FeTe<sub>2</sub>O<sub>8</sub>(OH)<sub>2</sub>(H<sub>2</sub>O)<sub>1+x</sub>.
Wolflehner, Tobias; Stöger, Berthold; Acta crystallographica Section B, Structural science, crystal engineering and materials 79 (2023) 510–518; doi:10.1107/S2052520623009162

data_2312335
_publ_section_title
;
 Order-disorder (OD) polytypism of
 K<sub>3</sub>FeTe<sub>2</sub>O<sub>8</sub>(OH)<sub>2</sub>(H<sub>2</sub>O)<sub>1+x</sub>.
;
_journal_coeditor_code           YV5013
_journal_issue                   6
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_page_first              510
_journal_page_last               518
_journal_paper_doi               10.1107/S2052520623009162
_journal_volume                  79
_journal_year                    2023
_chemical_formula_sum            'Fe H6 K3 O12 Te2'
_chemical_formula_weight         626.40
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-I 2y'
_space_group_name_H-M_alt        'I 1 2/m 1'
_atom_sites_solution_hydrogens   difmap
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90.002(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.8036(6)
_cell_length_b                   14.9042(8)
_cell_length_c                   5.9782(3)
_cell_measurement_reflns_used    4769
_cell_measurement_temperature    300
_cell_measurement_theta_max      36.04
_cell_measurement_theta_min      2.73
_cell_volume                     1140.80(10)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      300
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.961
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Bruker KAPPA APEX II CCD'
_diffrn_measurement_method       '\w- and \f-scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0280
_diffrn_reflns_av_unetI/netI     0.0284
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.961
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            9677
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.961
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         36.148
_diffrn_reflns_theta_min         2.733
_exptl_absorpt_coefficient_mu    7.487
_exptl_absorpt_correction_T_max  0.344
_exptl_absorpt_correction_T_min  0.261
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_density_diffrn    3.647
_exptl_crystal_description       needle
_exptl_crystal_F_000             1156
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.12
_refine_diff_density_max         1.331
_refine_diff_density_min         -0.960
_refine_diff_density_rms         0.179
_refine_ls_extinction_coef       0.00039(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.012
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_parameters     98
_refine_ls_number_reflns         2649
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.011
_refine_ls_R_factor_all          0.0259
_refine_ls_R_factor_gt           0.0204
_refine_ls_shift/su_max          0.015
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0219P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0431
_refine_ls_wR_factor_ref         0.0446
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2347
_reflns_number_total             2649
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            yv5013sup1.cif
_cod_data_source_block           300K
_cod_depositor_comments
'Adding full bibliography for 2312335--2312336.cif.'
_cod_original_sg_symbol_H-M      'I 2/m'
_cod_database_code               2312335
_cod_database_fobs_code          2312335
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.198
_shelx_estimated_absorpt_t_max   0.467
_shelx_res_checksum              63547
_shelx_hkl_checksum              54748